#------------------------------------------------------------------------------
#$Date: 2015-07-11 00:33:40 +0300 (Sat, 11 Jul 2015) $
#$Revision: 143561 $
#$URL: svn://www.crystallography.net/cod/cif/7/03/52/7035270.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7035270
loop_
_publ_author_name
'Li, Lu-Lu'
'Han, Hua-Yan'
'Wang, Yong-Hui'
'Tan, Hua-Qiao'
'Zang, Hong-Ying'
'Li, Yang-Guang'
_publ_section_title
;
 Construction of polyoxometalates from dynamic lacunary polyoxotungstate
 building blocks and lanthanide linkers.
;
_journal_issue                   25
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              11429
_journal_page_last               11436
_journal_paper_doi               10.1039/c5dt00686d
_journal_volume                  44
_journal_year                    2015
_chemical_formula_sum            'C12 H134 Dy4 Li15 N2 Na9 O207 Sb10 W36'
_chemical_formula_weight         12416.31
_chemical_name_systematic
;
 ?
;
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2014
_audit_update_record
;
2015-05-06 deposited with the CCDC.
2015-05-11 downloaded from the CCDC.
;
_cell_angle_alpha                101.760(2)
_cell_angle_beta                 107.002(2)
_cell_angle_gamma                105.855(2)
_cell_formula_units_Z            1
_cell_length_a                   14.1382(15)
_cell_length_b                   20.272(2)
_cell_length_c                   20.946(2)
_cell_measurement_reflns_used    39523
_cell_measurement_temperature    298(2)
_cell_measurement_theta_max      28.3575
_cell_measurement_theta_min      2.2495
_cell_volume                     5253.4(9)
_computing_cell_refinement       'SAINT (Bruker, 1999)'
_computing_data_collection       'SMART (Bruker, 1997)'
_computing_data_reduction        SAINT
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_diffrn_ambient_temperature      298(2)
_diffrn_measured_fraction_theta_full 0.970
_diffrn_measured_fraction_theta_max 0.995
_diffrn_measurement_device_type  'Bruker APEX CCD area-detector'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0639
_diffrn_reflns_av_unetI/netI     0.1169
_diffrn_reflns_laue_measured_fraction_full 0.970
_diffrn_reflns_laue_measured_fraction_max 0.995
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_k_max       21
_diffrn_reflns_limit_k_min       -24
_diffrn_reflns_limit_l_max       24
_diffrn_reflns_limit_l_min       -23
_diffrn_reflns_number            30044
_diffrn_reflns_point_group_measured_fraction_full 0.970
_diffrn_reflns_point_group_measured_fraction_max 0.995
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         25.000
_diffrn_reflns_theta_min         1.611
_diffrn_source                   'fine-focus sealed tube'
_exptl_absorpt_coefficient_mu    22.413
_exptl_absorpt_correction_T_max  0.089
_exptl_absorpt_correction_T_min  0.068
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Sheldrick, 1996)'
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    3.925
_exptl_crystal_description       block
_exptl_crystal_F_000             5458
_exptl_crystal_size_max          0.260
_exptl_crystal_size_mid          0.240
_exptl_crystal_size_min          0.210
_platon_squeeze_details
;
;
_refine_diff_density_max         8.069
_refine_diff_density_min         -11.416
_refine_diff_density_rms         0.600
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.056
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     1023
_refine_ls_number_reflns         18422
_refine_ls_number_restraints     570
_refine_ls_restrained_S_all      1.138
_refine_ls_R_factor_all          0.0807
_refine_ls_R_factor_gt           0.0653
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0700P)²] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1658
_refine_ls_wR_factor_ref         0.1735
_reflns_Friedel_coverage         0.000
_reflns_number_gt                13627
_reflns_number_total             18422
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            c5dt00686d2.cif
_cod_data_source_block           dy-4
_cod_depositor_comments
'Adding full bibliography for 7035268--7035272.cif.'
_cod_original_cell_volume        5253.4(10)
_cod_database_code               7035270
_audit_block_doi                 10.5517/cc13z4rz
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.068
_shelx_estimated_absorpt_t_max   0.089
_shelxl_version_number           2014-3
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
W1 W 0.07716(10) 0.47150(6) 0.69451(6) 0.0406(3) Uani 1 1 d . U .
W2 W -0.12569(10) 0.40988(5) 0.74351(6) 0.0365(3) Uani 1 1 d . . .
W3 W 0.11994(10) 0.47461(5) 0.86405(5) 0.0361(3) Uani 1 1 d . . .
W4 W 0.26731(9) 0.37698(5) 0.68500(5) 0.0350(3) Uani 1 1 d . . .
W5 W 0.31401(8) 0.38611(5) 0.85501(5) 0.0316(2) Uani 1 1 d . . .
W6 W -0.01521(9) 0.29305(5) 0.56293(5) 0.0317(2) Uani 1 1 d . U .
W7 W -0.23500(8) 0.25574(5) 0.79774(5) 0.0258(2) Uani 1 1 d . . .
W8 W -0.20088(8) 0.22531(5) 0.62426(5) 0.0261(2) Uani 1 1 d . . .
W9 W 0.24799(7) 0.22890(5) 0.73716(5) 0.0219(2) Uani 1 1 d . U .
W10 W -0.12848(7) -0.25225(4) 0.81422(4) 0.0186(2) Uani 1 1 d . . .
W11 W -0.02806(7) 0.14267(5) 0.61155(4) 0.0197(2) Uani 1 1 d . U .
W12 W -0.14366(6) -0.08977(4) 1.01948(4) 0.01235(18) Uiso 1 1 d . . .
W13 W -0.38408(6) -0.06111(5) 0.73588(4) 0.01651(19) Uani 1 1 d . . .
W14 W -0.36407(7) -0.22254(5) 0.69951(4) 0.0199(2) Uani 1 1 d . . .
W15 W -0.34829(6) -0.05434(5) 0.92569(4) 0.01511(19) Uani 1 1 d . U .
W16 W -0.33829(6) -0.21946(4) 0.87863(4) 0.0179(2) Uani 1 1 d . U .
W17 W 0.03540(6) -0.12020(4) 0.78358(4) 0.01511(19) Uani 1 1 d . U .
W18 W -0.20211(6) -0.08959(4) 0.67013(4) 0.01470(19) Uani 1 1 d . U .
Sb1 Sb 0.04531(11) 0.29568(7) 0.76161(7) 0.0199(3) Uani 1 1 d . U .
Sb2 Sb -0.13418(10) -0.05675(7) 0.85653(6) 0.0111(3) Uani 1 1 d . U .
Sb3 Sb -0.00044(11) 0.20765(7) 0.91118(7) 0.0167(3) Uani 1 1 d . . .
Sb4 Sb -0.18523(11) 0.08921(8) 0.73619(7) 0.0188(3) Uani 1 1 d . . .
Sb5 Sb -0.27301(11) 0.10379(7) 0.87504(7) 0.0172(3) Uani 1 1 d . . .
Dy1 Dy 0.06427(7) 0.07804(5) 0.77815(5) 0.0131(2) Uani 1 1 d . U .
Dy2 Dy 0.08815(7) -0.11589(5) 0.96013(5) 0.0144(2) Uani 1 1 d . U .
O1 O -0.1716(12) -0.3466(7) 0.7830(8) 0.026(4) Uani 1 1 d . U .
O2 O 0.1222(11) -0.1574(7) 1.0662(7) 0.019(3) Uani 1 1 d . U .
O3 O -0.2729(10) -0.0565(7) 1.0115(7) 0.017(3) Uani 1 1 d . U .
O4 O -0.3194(11) -0.1823(7) 0.6317(7) 0.021(3) Uani 1 1 d . U .
O5 O -0.3899(10) -0.0600(7) 0.8241(7) 0.015(3) Uani 1 1 d . U .
O6 O -0.3213(10) -0.0497(7) 0.6679(7) 0.019(3) Uani 1 1 d . U .
O7 O -0.2418(11) 0.1610(7) 0.8001(7) 0.020(3) Uani 1 1 d . U .
O8 O -0.1045(10) -0.1281(7) 0.7024(7) 0.015(3) Uani 1 1 d . U .
O9 O -0.1967(11) -0.0829(8) 0.5906(7) 0.022(3) Uani 1 1 d . U .
O10 O -0.1675(13) 0.2603(9) 0.5515(9) 0.037(4) Uani 1 1 d . U .
O11 O -0.0488(11) 0.1377(7) 0.8195(7) 0.023(3) Uani 1 1 d . U .
O12 O -0.4207(11) -0.1588(8) 0.8920(8) 0.022(3) Uani 1 1 d . U .
O13 O 0.1209(11) 0.1844(7) 0.6507(8) 0.022(3) Uani 1 1 d . U .
O14 O -0.1178(11) 0.0047(8) 0.7309(7) 0.021(3) Uani 1 1 d . U .
O15 O -0.0467(11) -0.2281(7) 0.7606(8) 0.023(3) Uani 1 1 d . U .
O16 O -0.2566(10) 0.0342(7) 0.7987(7) 0.014(3) Uani 1 1 d . U .
O17 O 0.1289(11) 0.1049(7) 0.8989(8) 0.023(3) Uani 1 1 d . U .
O18 O -0.0726(10) -0.1313(7) 0.8466(7) 0.013(3) Uani 1 1 d . U .
O19 O -0.1499(13) 0.3478(9) 0.8004(8) 0.033(4) Uani 1 1 d . U .
O20 O -0.2290(10) -0.2439(7) 0.8596(7) 0.018(3) Uani 1 1 d . U .
O21 O 0.0793(12) 0.0174(8) 0.6777(7) 0.026(4) Uani 1 1 d . U .
O22 O 0.1840(12) 0.3203(8) 0.7524(8) 0.027(4) Uani 1 1 d . U .
O23 O -0.2485(11) -0.1068(7) 0.7626(7) 0.021(3) Uani 1 1 d . U .
O24 O -0.3894(10) -0.2224(8) 0.7810(7) 0.022(3) Uani 1 1 d . U .
O25 O -0.0289(10) 0.1232(7) 0.6898(7) 0.020(3) Uani 1 1 d . U .
O26 O -0.4575(10) -0.1574(7) 0.6903(7) 0.016(3) Uani 1 1 d . U .
O27 O -0.2225(10) -0.1025(7) 0.9058(7) 0.017(3) Uani 1 1 d . U .
O28 O 0.1769(12) 0.1899(9) 0.7861(8) 0.031(4) Uani 1 1 d . U .
O29 O -0.0686(13) 0.4607(10) 0.6915(9) 0.041(4) Uani 1 1 d . U .
O30 O -0.1760(11) 0.2191(8) 0.7122(8) 0.024(3) Uani 1 1 d . U .
O31 O -0.2600(11) -0.1891(7) 0.9746(7) 0.019(3) Uani 1 1 d . U .
O32 O -0.0537(9) -0.1247(7) 0.9958(7) 0.010(3) Uani 1 1 d . U .
O33 O -0.0243(13) 0.1954(8) 0.5404(8) 0.032(4) Uani 1 1 d . U .
O34 O -0.4256(11) -0.3033(8) 0.8718(8) 0.027(4) Uani 1 1 d . U .
O35 O 0.0830(12) 0.4093(8) 0.9044(8) 0.029(4) Uani 1 1 d . U .
O36 O -0.0211(10) -0.2353(7) 0.8938(7) 0.020(3) Uani 1 1 d . U .
O37 O -0.0461(12) 0.0625(9) 0.5534(8) 0.034(4) Uani 1 1 d . U .
O38 O -0.2414(9) 0.0366(7) 0.9373(6) 0.015(3) Uani 1 1 d . U .
O39 O -0.4583(12) -0.3017(8) 0.6404(8) 0.029(4) Uani 1 1 d . U .
O40 O -0.4789(12) -0.0239(8) 0.7077(7) 0.028(4) Uani 1 1 d . U .
O41 O -0.0759(11) 0.0051(8) 1.0379(8) 0.023(3) Uani 1 1 d . U .
O42 O 0.1311(9) -0.1181(7) 0.8622(7) 0.013(3) Uani 1 1 d . U .
O43 O 0.1927(14) 0.4440(9) 0.6995(9) 0.042(4) Uani 1 1 d . U .
O44 O -0.2578(11) -0.2508(8) 0.7304(8) 0.026(4) Uani 1 1 d . U .
O45 O 0.1347(13) 0.3222(8) 0.6077(8) 0.033(4) Uani 1 1 d . U .
O46 O 0.0316(11) 0.3894(8) 0.7592(8) 0.025(3) Uani 1 1 d . U .
O47 O -0.0281(11) 0.2552(8) 0.6574(7) 0.023(3) Uani 1 1 d . U .
O48 O 0.3534(13) 0.4227(9) 0.7766(8) 0.037(4) Uani 1 1 d . U .
O49 O -0.3537(14) 0.2413(9) 0.7320(9) 0.041(5) Uani 1 1 d . U .
O50 O -0.1765(12) 0.1380(8) 0.5884(8) 0.030(4) Uani 1 1 d . U .
O51 O 0.4306(13) 0.4381(9) 0.9238(9) 0.039(4) Uani 1 1 d . U .
O52 O -0.2620(14) 0.2807(10) 0.8708(9) 0.044(5) Uani 1 1 d . U .
O53 O 0.3546(13) 0.3037(9) 0.8139(9) 0.035(4) Uani 1 1 d . U .
O54 O 0.2972(13) 0.2938(9) 0.6788(8) 0.035(4) Uani 1 1 d . U .
O55 O 0.0993(12) -0.1337(8) 0.7228(7) 0.024(3) Uani 1 1 d . U .
O56 O -0.4487(12) -0.0283(9) 0.9419(8) 0.031(4) Uani 1 1 d . U .
O57 O 0.3361(15) 0.4162(10) 0.6403(10) 0.049(5) Uani 1 1 d . U .
O58 O -0.0684(12) 0.2741(7) 0.8733(8) 0.024(3) Uani 1 1 d . U .
O59 O 0.1428(16) 0.5217(9) 0.7896(9) 0.051(5) Uani 1 1 d . U .
O60 O -0.0221(13) 0.4771(10) 0.8324(10) 0.046(5) Uani 1 1 d . U .
O61 O -0.0268(16) 0.3064(10) 0.4832(10) 0.054(5) Uani 1 1 d . U .
O62 O -0.3375(12) 0.1912(9) 0.5824(8) 0.036(4) Uani 1 1 d . U .
O63 O 0.3200(12) 0.1749(9) 0.7196(9) 0.035(4) Uani 1 1 d . U .
O64 O 0.2416(14) 0.3367(9) 0.8938(9) 0.040(4) Uani 1 1 d . U .
O65 O -0.1752(14) 0.3285(9) 0.6643(9) 0.039(4) Uani 1 1 d . U .
O66 O -0.2257(17) 0.4387(10) 0.7379(10) 0.054(5) Uani 1 1 d . U .
O67 O 0.1818(16) 0.5555(10) 0.9342(10) 0.053(5) Uani 1 1 d . U .
O68 O 0.2412(16) 0.4546(10) 0.8548(10) 0.052(5) Uani 1 1 d . U .
O69 O -0.0072(14) 0.3835(9) 0.6141(10) 0.043(5) Uani 1 1 d . U .
O70 O 0.1694(16) -0.0204(11) 0.6176(10) 0.054(5) Uani 1 1 d . U .
O71 O 0.0935(19) 0.5370(12) 0.6509(12) 0.072(7) Uani 1 1 d . U .
O72 O 0.0503(10) -0.0273(7) 0.8023(7) 0.013(3) Uani 1 1 d . U .
O1W O 0.2264(12) -0.1728(8) 0.9734(8) 0.029(4) Uani 1 1 d . U .
N1 N 0.2400(9) 0.0617(7) 0.7974(6) 0.019(3) Uani 1 1 d G U .
C1 C 0.3179(10) 0.0808(7) 0.8634(7) 0.026(4) Uani 1 1 d G U .
H1 H 0.3134 0.1096 0.9023 0.026 Uiso 1 1 calc R U .
C2 C 0.4026(11) 0.0569(8) 0.8713(7) 0.031(5) Uani 1 1 d G U .
H2 H 0.4548 0.0697 0.9154 0.031 Uiso 1 1 calc R U .
C3 C 0.4094(11) 0.0139(9) 0.8132(8) 0.034(5) Uani 1 1 d G U .
H3 H 0.4661 -0.0022 0.8185 0.034 Uiso 1 1 calc R U .
C4 C 0.3315(12) -0.0052(9) 0.7472(7) 0.042(5) Uani 1 1 d G U .
H4 H 0.3360 -0.0340 0.7084 0.042 Uiso 1 1 calc R U .
C5 C 0.2467(10) 0.0187(8) 0.7393(7) 0.025(4) Uani 1 1 d G U .
C6 C 0.1597(17) 0.0052(12) 0.6746(11) 0.024(5) Uani 1 1 d . U .
Na1 Na -0.0384(8) -0.0520(5) 0.5558(5) 0.042(3) Uani 1 1 d . U .
Na2 Na 0.1695(13) 0.4312(9) 1.0368(9) 0.065(5) Uiso 0.75 1 d . . P
Na3 Na -0.3600(16) -0.2510(11) 1.0537(11) 0.084(6) Uiso 0.75 1 d . . P
Na4 Na 0.3348(19) -0.1179(13) 0.8939(14) 0.061(7) Uiso 0.5 1 d . . P
Na5 Na -0.1852(18) 0.3100(12) 1.0116(12) 0.053(6) Uiso 0.5 1 d . . P
Na6 Na 0.564(2) 0.5465(16) 0.9532(16) 0.080(8) Uiso 0.5 1 d . . P
Na7 Na 0.327(2) 0.1262(16) 0.5298(16) 0.082(9) Uiso 0.5 1 d . . P
O2W O 0.0339(16) 0.1663(11) 0.4244(11) 0.059(6) Uiso 1 1 d . . .
O3W O -0.2541(18) -0.4550(13) 0.8344(13) 0.074(7) Uiso 1 1 d . . .
O4W O 0.181(2) 0.0865(14) 0.5572(14) 0.089(8) Uiso 1 1 d . . .
O5W O -0.0327(17) -0.3295(12) 0.9700(12) 0.064(6) Uiso 1 1 d . . .
O6W O 0.329(3) 0.531(2) 1.047(2) 0.062(12) Uiso 0.5 1 d . . P
O7W O 0.266(2) -0.1100(16) 0.5713(16) 0.067(8) Uiso 0.75 1 d . . P
O8W O 0.270(2) 0.3525(15) 1.0288(15) 0.098(9) Uiso 1 1 d . . .
O9W O 0.535(3) 0.5362(19) 0.8300(19) 0.085(10) Uiso 0.75 1 d . . P
O10W O -0.559(3) -0.222(2) 0.963(2) 0.101(12) Uiso 0.75 1 d . . P
O11W O 0.104(3) 0.523(2) 1.060(2) 0.082(11) Uiso 0.65 1 d . . P
O12W O -0.619(3) -0.2083(19) 0.7665(19) 0.087(10) Uiso 0.75 1 d . . P
O13W O -0.453(3) -0.185(2) 0.511(2) 0.052(10) Uiso 0.5 1 d . . P
O14W O -0.174(4) -0.289(3) 0.601(3) 0.083(15) Uiso 0.5 1 d . . P
O15W O -0.492(6) 0.100(4) 0.653(4) 0.09(2) Uiso 0.35 1 d . . P
O16W O -0.326(3) -0.014(2) 0.511(2) 0.050(10) Uiso 0.5 1 d . . P
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sb Sb -0.5866 1.5461 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Dy Dy -0.1892 4.4098 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Li Li -0.0003 0.0001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O71 W1 O43 102.7(10) . .
O71 W1 O59 105.8(9) . .
O43 W1 O59 88.8(9) . .
O71 W1 O69 100.7(9) . .
O43 W1 O69 87.3(7) . .
O59 W1 O69 153.5(8) . .
O71 W1 O29 98.5(10) . .
O43 W1 O29 156.6(8) . .
O59 W1 O29 94.9(8) . .
O69 W1 O29 79.1(8) . .
O71 W1 O46 169.8(9) . .
O43 W1 O46 87.2(7) . .
O59 W1 O46 71.7(6) . .
O69 W1 O46 81.9(7) . .
O29 W1 O46 72.2(7) . .
O66 W2 O29 97.7(9) . .
O66 W2 O65 106.0(9) . .
O29 W2 O65 85.8(8) . .
O66 W2 O19 99.2(9) . .
O29 W2 O19 163.0(7) . .
O65 W2 O19 90.0(7) . .
O66 W2 O60 100.2(8) . .
O29 W2 O60 93.5(8) . .
O65 W2 O60 153.6(7) . .
O19 W2 O60 83.0(8) . .
O66 W2 O46 170.6(8) . .
O29 W2 O46 77.3(7) . .
O65 W2 O46 81.8(7) . .
O19 W2 O46 85.9(6) . .
O60 W2 O46 72.4(6) . .
O67 W3 O35 103.3(8) . .
O67 W3 O68 100.6(9) . .
O35 W3 O68 96.7(8) . .
O67 W3 O60 98.8(9) . .
O35 W3 O60 91.5(8) . .
O68 W3 O60 156.5(8) . .
O67 W3 O59 95.2(8) . .
O35 W3 O59 161.5(7) . .
O68 W3 O59 78.7(9) . .
O60 W3 O59 86.5(9) . .
O67 W3 O46 165.9(8) . .
O35 W3 O46 89.1(6) . .
O68 W3 O46 84.2(7) . .
O60 W3 O46 74.0(6) . .
O59 W3 O46 72.7(6) . .
O57 W4 O48 103.8(9) . .
O57 W4 O54 101.1(9) . .
O48 W4 O54 96.1(7) . .
O57 W4 O45 98.6(8) . .
O48 W4 O45 155.8(8) . .
O54 W4 O45 88.4(7) . .
O57 W4 O43 99.1(9) . .
O48 W4 O43 85.7(8) . .
O54 W4 O43 158.7(7) . .
O45 W4 O43 81.9(7) . .
O57 W4 O22 175.2(8) . .
O48 W4 O22 73.4(7) . .
O54 W4 O22 75.6(6) . .
O45 W4 O22 84.9(6) . .
O43 W4 O22 84.6(6) . .
O51 W5 O64 103.1(9) . .
O51 W5 O68 99.3(8) . .
O64 W5 O68 93.8(9) . .
O51 W5 O53 100.3(7) . .
O64 W5 O53 93.6(8) . .
O68 W5 O53 156.9(7) . .
O51 W5 O48 97.5(8) . .
O64 W5 O48 159.4(7) . .
O68 W5 O48 83.9(8) . .
O53 W5 O48 81.6(7) . .
O51 W5 O22 168.0(8) . .
O64 W5 O22 87.4(7) . .
O68 W5 O22 85.7(7) . .
O53 W5 O22 72.9(6) . .
O48 W5 O22 72.0(6) . .
O51 W5 Na6 36.9(8) . 2_667
O64 W5 Na6 67.9(8) . 2_667
O68 W5 Na6 90.7(7) . 2_667
O53 W5 Na6 112.4(6) . 2_667
O48 W5 Na6 132.5(7) . 2_667
O22 W5 Na6 154.8(7) . 2_667
O61 W6 O69 100.1(9) . .
O61 W6 O33 99.6(8) . .
O69 W6 O33 160.2(8) . .
O61 W6 O45 101.5(9) . .
O69 W6 O45 88.8(7) . .
O33 W6 O45 89.3(7) . .
O61 W6 O10 99.6(9) . .
O69 W6 O10 85.4(7) . .
O33 W6 O10 89.2(7) . .
O45 W6 O10 158.7(7) . .
O61 W6 O47 168.8(7) . .
O69 W6 O47 87.0(7) . .
O33 W6 O47 73.2(6) . .
O45 W6 O47 87.1(6) . .
O10 W6 O47 72.2(6) . .
O52 W7 O49 101.4(9) . .
O52 W7 O19 99.3(8) . .
O49 W7 O19 101.3(8) . .
O52 W7 O7 97.2(8) . .
O49 W7 O7 103.7(7) . .
O19 W7 O7 146.5(6) . .
O52 W7 O30 170.4(7) . .
O49 W7 O30 87.8(7) . .
O19 W7 O30 81.4(6) . .
O7 W7 O30 77.7(6) . .
O52 W7 O58 86.1(7) . .
O49 W7 O58 172.3(8) . .
O19 W7 O58 75.6(6) . .
O7 W7 O58 76.7(5) . .
O30 W7 O58 84.8(5) . .
O62 W8 O30 105.5(7) . .
O62 W8 O10 97.4(8) . .
O30 W8 O10 155.8(7) . .
O62 W8 O50 97.0(7) . .
O30 W8 O50 95.2(7) . .
O10 W8 O50 89.6(7) . .
O62 W8 O65 101.0(8) . .
O30 W8 O65 87.2(7) . .
O10 W8 O65 80.8(7) . .
O50 W8 O65 160.5(7) . .
O62 W8 O47 168.4(7) . .
O30 W8 O47 82.9(6) . .
O10 W8 O47 75.6(6) . .
O50 W8 O47 73.9(6) . .
O65 W8 O47 87.3(7) . .
O63 W9 O28 106.0(8) . .
O63 W9 O53 99.4(7) . .
O28 W9 O53 96.2(7) . .
O63 W9 O13 99.9(7) . .
O28 W9 O13 91.1(7) . .
O53 W9 O13 156.6(6) . .
O63 W9 O54 92.8(8) . .
O28 W9 O54 160.8(7) . .
O53 W9 O54 84.0(7) . .
O13 W9 O54 81.9(6) . .
O63 W9 O22 165.0(7) . .
O28 W9 O22 88.4(7) . .
O53 W9 O22 74.3(6) . .
O13 W9 O22 83.7(5) . .
O54 W9 O22 73.2(6) . .
O1 W10 O36 99.9(7) . .
O1 W10 O15 100.0(7) . .
O36 W10 O15 97.1(6) . .
O1 W10 O20 98.5(7) . .
O36 W10 O20 95.0(6) . .
O15 W10 O20 155.8(6) . .
O1 W10 O44 91.3(6) . .
O36 W10 O44 167.7(6) . .
O15 W10 O44 85.9(6) . .
O20 W10 O44 78.1(6) . .
O1 W10 O18 175.8(6) . .
O36 W10 O18 82.7(5) . .
O15 W10 O18 76.3(5) . .
O20 W10 O18 84.5(5) . .
O44 W10 O18 86.5(5) . .
O1 W10 Dy2 134.5(5) . .
O36 W10 Dy2 34.9(4) . .
O15 W10 Dy2 85.9(4) . .
O20 W10 Dy2 92.2(4) . .
O44 W10 Dy2 134.2(4) . .
O18 W10 Dy2 47.8(3) . .
O37 W11 O25 105.6(8) . .
O37 W11 O13 101.0(7) . .
O25 W11 O13 90.2(6) . .
O37 W11 O50 100.6(7) . .
O25 W11 O50 89.3(6) . .
O13 W11 O50 157.7(6) . .
O37 W11 O33 92.6(7) . .
O25 W11 O33 161.7(6) . .
O13 W11 O33 87.7(7) . .
O50 W11 O33 85.8(7) . .
O37 W11 O47 162.5(7) . .
O25 W11 O47 90.0(6) . .
O13 W11 O47 86.5(5) . .
O50 W11 O47 71.2(5) . .
O33 W11 O47 71.7(6) . .
O17 W12 O32 101.3(6) 2_557 .
O17 W12 O41 106.7(7) 2_557 .
O32 W12 O41 100.4(6) . .
O17 W12 O31 87.3(6) 2_557 .
O32 W12 O31 90.8(6) . .
O41 W12 O31 159.8(6) . .
O17 W12 O3 96.1(6) 2_557 .
O32 W12 O3 160.9(6) . .
O41 W12 O3 81.8(6) . .
O31 W12 O3 82.2(5) . .
O17 W12 O27 158.1(6) 2_557 .
O32 W12 O27 87.5(5) . .
O41 W12 O27 91.1(6) . .
O31 W12 O27 72.4(5) . .
O3 W12 O27 73.5(5) . .
O40 W13 O26 102.1(6) . .
O40 W13 O5 99.0(6) . .
O26 W13 O5 98.1(6) . .
O40 W13 O6 97.5(7) . .
O26 W13 O6 93.0(6) . .
O5 W13 O6 157.6(5) . .
O40 W13 O16 98.6(6) . .
O26 W13 O16 159.3(5) . .
O5 W13 O16 79.9(5) . .
O6 W13 O16 82.8(5) . .
O40 W13 O23 172.4(7) . .
O26 W13 O23 79.3(5) . .
O5 W13 O23 88.1(5) . .
O6 W13 O23 75.0(5) . .
O16 W13 O23 80.0(5) . .
O39 W14 O44 100.9(7) . .
O39 W14 O24 102.8(7) . .
O44 W14 O24 89.6(7) . .
O39 W14 O4 96.9(7) . .
O44 W14 O4 97.5(7) . .
O24 W14 O4 157.4(6) . .
O39 W14 O26 98.0(7) . .
O44 W14 O26 160.8(6) . .
O24 W14 O26 83.2(6) . .
O4 W14 O26 83.2(6) . .
O39 W14 O23 169.2(7) . .
O44 W14 O23 87.0(6) . .
O24 W14 O23 84.4(6) . .
O4 W14 O23 74.6(5) . .
O26 W14 O23 74.6(5) . .
O56 W15 O3 101.8(7) . .
O56 W15 O12 99.2(7) . .
O3 W15 O12 92.2(6) . .
O56 W15 O38 103.5(7) . .
O3 W15 O38 91.5(6) . .
O12 W15 O38 155.7(6) . .
O56 W15 O5 98.1(6) . .
O3 W15 O5 160.0(6) . .
O12 W15 O5 85.9(6) . .
O38 W15 O5 82.5(5) . .
O56 W15 O27 173.2(7) . .
O3 W15 O27 75.8(5) . .
O12 W15 O27 74.6(5) . .
O38 W15 O27 83.0(5) . .
O5 W15 O27 84.5(5) . .
O34 W16 O31 98.6(7) . .
O34 W16 O20 102.1(6) . .
O31 W16 O20 90.6(6) . .
O34 W16 O24 99.2(7) . .
O31 W16 O24 162.1(6) . .
O20 W16 O24 85.5(6) . .
O34 W16 O12 100.7(7) . .
O31 W16 O12 91.4(6) . .
O20 W16 O12 156.5(6) . .
O24 W16 O12 85.5(6) . .
O34 W16 O27 170.8(6) . .
O31 W16 O27 73.5(6) . .
O20 W16 O27 83.0(5) . .
O24 W16 O27 88.7(6) . .
O12 W16 O27 75.2(5) . .
O55 W17 O42 101.3(6) . .
O55 W17 O72 104.4(7) . .
O42 W17 O72 100.5(6) . .
O55 W17 O15 94.4(6) . .
O42 W17 O15 92.3(6) . .
O72 W17 O15 154.6(6) . .
O55 W17 O8 91.7(6) . .
O42 W17 O8 166.3(6) . .
O72 W17 O8 80.3(5) . .
O15 W17 O8 82.1(5) . .
O55 W17 O18 166.0(6) . .
O42 W17 O18 83.3(5) . .
O72 W17 O18 87.6(5) . .
O15 W17 O18 72.1(5) . .
O8 W17 O18 83.1(5) . .
O55 W17 Dy2 135.6(5) . .
O42 W17 Dy2 34.7(4) . .
O72 W17 Dy2 93.3(4) . .
O15 W17 Dy2 84.8(4) . .
O8 W17 Dy2 131.8(4) . .
O18 W17 Dy2 48.8(3) . .
O9 W18 O8 104.7(6) . .
O9 W18 O14 102.3(7) . .
O8 W18 O14 94.4(6) . .
O9 W18 O4 95.9(6) . .
O8 W18 O4 93.7(6) . .
O14 W18 O4 157.5(6) . .
O9 W18 O6 97.1(6) . .
O8 W18 O6 158.1(6) . .
O14 W18 O6 81.9(6) . .
O4 W18 O6 82.7(6) . .
O9 W18 O23 167.4(6) . .
O8 W18 O23 84.8(6) . .
O14 W18 O23 84.9(6) . .
O4 W18 O23 74.9(5) . .
O6 W18 O23 73.4(6) . .
O22 Sb1 O46 94.7(6) . .
O22 Sb1 O47 90.9(6) . .
O46 Sb1 O47 90.8(6) . .
O18 Sb2 O23 92.1(5) . .
O18 Sb2 O27 93.8(6) . .
O23 Sb2 O27 93.1(6) . .
O11 Sb3 O2 94.2(6) . 2_557
O11 Sb3 O58 93.6(6) . .
O2 Sb3 O58 94.2(6) 2_557 .
O11 Sb4 O16 89.9(6) . .
O11 Sb4 O14 79.2(5) . .
O16 Sb4 O14 82.0(5) . .
O11 Sb4 O7 83.1(5) . .
O16 Sb4 O7 69.4(5) . .
O14 Sb4 O7 146.3(5) . .
O11 Sb4 Dy1 45.2(4) . .
O16 Sb4 Dy1 105.2(3) . .
O14 Sb4 Dy1 42.7(4) . .
O7 Sb4 Dy1 128.3(3) . .
O2 Sb5 O16 99.1(5) 2_557 .
O2 Sb5 O38 78.7(5) 2_557 .
O16 Sb5 O38 86.6(5) . .
O2 Sb5 O7 85.5(6) 2_557 .
O16 Sb5 O7 72.9(5) . .
O38 Sb5 O7 151.8(5) . .
O2 Sb5 Dy2 42.1(4) 2_557 2_557
O16 Sb5 Dy2 107.8(4) . 2_557
O38 Sb5 Dy2 40.9(3) . 2_557
O7 Sb5 Dy2 127.6(4) . 2_557
O72 Dy1 O21 83.0(5) . .
O72 Dy1 O28 146.8(5) . .
O21 Dy1 O28 94.4(6) . .
O72 Dy1 O17 72.8(5) . .
O21 Dy1 O17 142.8(5) . .
O28 Dy1 O17 91.1(5) . .
O72 Dy1 O14 72.1(5) . .
O21 Dy1 O14 88.2(5) . .
O28 Dy1 O14 141.1(5) . .
O17 Dy1 O14 109.9(5) . .
O72 Dy1 O25 139.0(4) . .
O21 Dy1 O25 77.4(5) . .
O28 Dy1 O25 71.1(5) . .
O17 Dy1 O25 138.5(5) . .
O14 Dy1 O25 71.7(5) . .
O72 Dy1 O11 112.5(5) . .
O21 Dy1 O11 142.4(5) . .
O28 Dy1 O11 89.6(5) . .
O17 Dy1 O11 74.3(5) . .
O14 Dy1 O11 66.5(5) . .
O25 Dy1 O11 68.6(5) . .
O72 Dy1 N1 72.5(5) . .
O21 Dy1 N1 65.7(4) . .
O28 Dy1 N1 76.3(5) . .
O17 Dy1 N1 80.1(4) . .
O14 Dy1 N1 138.0(5) . .
O25 Dy1 N1 127.8(4) . .
O11 Dy1 N1 150.5(4) . .
O72 Dy1 Sb4 106.4(3) . .
O21 Dy1 Sb4 109.1(4) . .
O28 Dy1 Sb4 105.7(4) . .
O17 Dy1 Sb4 104.7(3) . .
O14 Dy1 Sb4 38.4(3) . .
O25 Dy1 Sb4 49.7(3) . .
O11 Dy1 Sb4 34.8(3) . .
N1 Dy1 Sb4 174.7(3) . .
O41 Dy2 O32 80.0(5) 2_557 .
O41 Dy2 O42 88.2(5) 2_557 .
O32 Dy2 O42 141.2(4) . .
O41 Dy2 O36 134.8(5) 2_557 .
O32 Dy2 O36 80.1(5) . .
O42 Dy2 O36 82.6(5) . .
O41 Dy2 O38 78.0(5) 2_557 2_557
O32 Dy2 O38 104.7(4) . 2_557
O42 Dy2 O38 108.8(4) . 2_557
O36 Dy2 O38 146.6(5) . 2_557
O41 Dy2 O2 123.0(5) 2_557 .
O32 Dy2 O2 71.7(5) . .
O42 Dy2 O2 142.0(4) . .
O36 Dy2 O2 87.8(5) . .
O38 Dy2 O2 63.7(5) 2_557 .
O41 Dy2 O1W 138.5(5) 2_557 .
O32 Dy2 O1W 135.4(5) . .
O42 Dy2 O1W 74.6(5) . .
O36 Dy2 O1W 81.0(5) . .
O38 Dy2 O1W 72.6(5) 2_557 .
O2 Dy2 O1W 67.5(5) . .
O41 Dy2 O18 71.1(5) 2_557 .
O32 Dy2 O18 74.7(4) . .
O42 Dy2 O18 66.4(4) . .
O36 Dy2 O18 64.6(4) . .
O38 Dy2 O18 148.8(4) 2_557 .
O2 Dy2 O18 139.5(4) . .
O1W Dy2 O18 130.1(4) . .
O41 Dy2 W17 77.5(4) 2_557 .
O32 Dy2 W17 115.1(3) . .
O42 Dy2 W17 26.2(3) . .
O36 Dy2 W17 75.0(4) . .
O38 Dy2 W17 128.0(3) 2_557 .
O2 Dy2 W17 159.4(3) . .
O1W Dy2 W17 98.2(4) . .
O18 Dy2 W17 40.4(3) . .
O41 Dy2 W10 109.6(4) 2_557 .
O32 Dy2 W10 76.9(3) . .
O42 Dy2 W10 72.5(3) . .
O36 Dy2 W10 25.9(3) . .
O38 Dy2 W10 172.4(3) 2_557 .
O2 Dy2 W10 110.5(3) . .
O1W Dy2 W10 101.0(3) . .
O18 Dy2 W10 38.8(3) . .
W17 Dy2 W10 55.95(2) . .
O41 Dy2 Sb5 109.9(4) 2_557 2_557
O32 Dy2 Sb5 96.2(3) . 2_557
O42 Dy2 Sb5 122.5(3) . 2_557
O36 Dy2 Sb5 112.4(3) . 2_557
O38 Dy2 Sb5 34.9(3) 2_557 2_557
O2 Dy2 Sb5 32.0(3) . 2_557
O1W Dy2 Sb5 55.4(3) . 2_557
O18 Dy2 Sb5 170.7(3) . 2_557
W17 Dy2 Sb5 148.65(4) . 2_557
W10 Dy2 Sb5 137.98(4) . 2_557
Sb5 O2 Sb3 131.8(7) 2_557 2_557
Sb5 O2 Dy2 106.0(6) 2_557 .
Sb3 O2 Dy2 119.2(6) 2_557 .
W15 O3 W12 117.1(7) . .
W14 O4 W18 116.4(7) . .
W13 O5 W15 162.0(7) . .
W13 O6 W18 117.1(7) . .
W7 O7 Sb5 131.0(7) . .
W7 O7 Sb4 125.4(7) . .
Sb5 O7 Sb4 102.6(6) . .
W18 O8 W17 148.8(7) . .
W18 O9 Na7 134.4(11) . 2_556
W18 O9 Na1 128.9(7) . .
Na7 O9 Na1 95.1(10) 2_556 .
W8 O10 W6 116.4(7) . .
Sb3 O11 Sb4 136.3(8) . .
Sb3 O11 Dy1 123.7(7) . .
Sb4 O11 Dy1 100.0(5) . .
W15 O12 W16 118.2(7) . .
W11 O13 W9 146.4(8) . .
W18 O14 Sb4 119.9(7) . .
W18 O14 Dy1 136.8(7) . .
Sb4 O14 Dy1 98.9(5) . .
W10 O15 W17 116.2(7) . .
Sb5 O16 W13 119.4(6) . .
Sb5 O16 Sb4 111.7(6) . .
W13 O16 Sb4 111.7(6) . .
W12 O17 Dy1 157.1(8) 2_557 .
Sb2 O18 W10 137.6(6) . .
Sb2 O18 W17 114.9(6) . .
W10 O18 W17 94.7(5) . .
Sb2 O18 Dy2 114.6(5) . .
W10 O18 Dy2 93.4(4) . .
W17 O18 Dy2 90.7(4) . .
W7 O19 W2 143.5(9) . .
W16 O20 W10 159.2(8) . .
C6 O21 Dy1 125.3(13) . .
C6 O21 Na1 97.2(13) . .
Dy1 O21 Na1 137.2(7) . .
Sb1 O22 W5 111.4(7) . .
Sb1 O22 W9 116.2(7) . .
W5 O22 W9 94.5(6) . .
Sb1 O22 W4 137.8(7) . .
W5 O22 W4 94.8(6) . .
W9 O22 W4 92.9(6) . .
Sb2 O23 W18 115.3(7) . .
Sb2 O23 W14 137.2(7) . .
W18 O23 W14 92.8(5) . .
Sb2 O23 W13 116.1(6) . .
W18 O23 W13 94.4(5) . .
W14 O23 W13 91.5(5) . .
W14 O24 W16 149.0(8) . .
W11 O25 Dy1 141.2(7) . .
W13 O26 W14 114.5(6) . .
Sb2 O27 W12 118.4(6) . .
Sb2 O27 W16 132.0(7) . .
W12 O27 W16 94.9(5) . .
Sb2 O27 W15 117.9(6) . .
W12 O27 W15 93.3(5) . .
W16 O27 W15 91.4(5) . .
W9 O28 Dy1 138.9(8) . .
W2 O29 W1 120.5(9) . .
W8 O30 W7 134.0(7) . .
W16 O31 W12 119.1(8) . .
W16 O31 Na3 115.6(7) . .
W12 O31 Na3 120.0(7) . .
W12 O32 Dy2 152.5(7) . .
W6 O33 W11 119.9(8) . .
W3 O35 Na2 122.4(8) . .
W10 O36 Dy2 119.2(7) . .
W11 O37 Na1 138.5(10) . .
W11 O37 Na1 124.3(9) . 2_556
Na1 O37 Na1 87.9(6) . 2_556
W15 O38 Sb5 122.4(6) . .
W15 O38 Dy2 129.5(6) . 2_557
Sb5 O38 Dy2 104.2(5) . 2_557
W12 O41 Dy2 147.7(8) . 2_557
W17 O42 Dy2 119.1(6) . .
W17 O42 Na4 132.1(9) . .
Dy2 O42 Na4 108.7(7) . .
W1 O43 W4 156.4(10) . .
W14 O44 W10 151.3(9) . .
W6 O45 W4 152.8(10) . .
Sb1 O46 W3 112.4(7) . .
Sb1 O46 W2 123.1(7) . .
W3 O46 W2 94.4(6) . .
Sb1 O46 W1 134.3(8) . .
W3 O46 W1 93.7(5) . .
W2 O46 W1 89.5(5) . .
Sb1 O47 W8 112.3(7) . .
Sb1 O47 W11 113.9(7) . .
W8 O47 W11 96.9(5) . .
Sb1 O47 W6 135.6(7) . .
W8 O47 W6 95.8(5) . .
W11 O47 W6 95.0(6) . .
W4 O48 W5 119.7(8) . .
W8 O50 W11 117.9(7) . .
W5 O51 Na6 137.7(13) . .
W5 O51 Na6 118.9(12) . 2_667
Na6 O51 Na6 94.3(13) . 2_667
W7 O52 Na5 143.2(10) . .
W9 O53 W5 116.4(8) . .
W4 O54 W9 118.1(9) . .
W15 O56 Na4 125.9(9) . 1_455
Sb3 O58 W7 133.1(7) . .
W1 O59 W3 121.7(9) . .
W3 O60 W2 119.2(8) . .
W5 O64 Na3 105.6(9) . 2_557
W2 O65 W8 149.3(10) . .
W3 O67 Na5 147.0(12) . 2_567
W3 O68 W5 146.1(12) . .
W6 O69 W1 147.1(10) . .
C6 O70 Na1 86.9(14) . .
W17 O72 Dy1 155.6(7) . .
Dy2 O1W Na4 102.6(7) . .
Dy2 O1W Na5 120.7(8) . 2_557
Na4 O1W Na5 126.7(9) . 2_557
C1 N1 C5 120.0 . .
C1 N1 Dy1 123.4(6) . .
C5 N1 Dy1 115.3(6) . .
C2 C1 N1 120.0 . .
C1 C2 C3 120.0 . .
C4 C3 C2 120.0 . .
C3 C4 C5 120.0 . .
C4 C5 N1 120.0 . .
C4 C5 C6 127.5(12) . .
N1 C5 C6 112.5(12) . .
O21 C6 O70 123(2) . .
O21 C6 C5 119.3(18) . .
O70 C6 C5 117.3(19) . .
O21 C6 Na1 57.5(11) . .
O70 C6 Na1 67.3(13) . .
C5 C6 Na1 165.6(16) . .
O37 Na1 O4W 80.2(8) . 2_556
O37 Na1 O2W 171.2(9) . 2_556
O4W Na1 O2W 104.7(9) 2_556 2_556
O37 Na1 O21 81.5(6) . .
O4W Na1 O21 159.3(9) 2_556 .
O2W Na1 O21 92.2(7) 2_556 .
O37 Na1 O9 92.0(6) . .
O4W Na1 O9 79.4(8) 2_556 .
O2W Na1 O9 81.9(7) 2_556 .
O21 Na1 O9 91.6(6) . .
O37 Na1 O70 101.6(7) . .
O4W Na1 O70 143.5(10) 2_556 .
O2W Na1 O70 78.9(7) 2_556 .
O21 Na1 O70 50.8(6) . .
O9 Na1 O70 136.3(7) . .
O37 Na1 O37 92.1(6) . 2_556
O4W Na1 O37 70.5(8) 2_556 2_556
O2W Na1 O37 96.4(7) 2_556 2_556
O21 Na1 O37 120.0(6) . 2_556
O9 Na1 O37 148.4(6) . 2_556
O70 Na1 O37 73.0(6) . 2_556
O37 Na1 C6 94.4(7) . .
O4W Na1 C6 167.0(10) 2_556 .
O2W Na1 C6 82.2(7) 2_556 .
O21 Na1 C6 25.3(6) . .
O9 Na1 C6 112.8(7) . .
O70 Na1 C6 25.9(6) . .
O37 Na1 C6 98.0(6) 2_556 .
O37 Na1 Na1 51.8(5) . 2_556
O4W Na1 Na1 68.1(8) 2_556 2_556
O2W Na1 Na1 136.6(8) 2_556 2_556
O21 Na1 Na1 107.3(6) . 2_556
O9 Na1 Na1 133.9(6) . 2_556
O70 Na1 Na1 84.2(6) . 2_556
O37 Na1 Na1 40.3(4) 2_556 2_556
C6 Na1 Na1 99.2(6) . 2_556
O37 Na1 Na7 88.0(7) . 2_556
O4W Na1 Na7 37.8(9) 2_556 2_556
O2W Na1 Na7 91.7(8) 2_556 2_556
O21 Na1 Na7 132.0(8) . 2_556
O9 Na1 Na7 41.9(6) . 2_556
O70 Na1 Na7 170.5(8) . 2_556
O37 Na1 Na7 107.1(7) 2_556 2_556
C6 Na1 Na7 154.7(8) . 2_556
Na1 Na1 Na7 102.0(6) 2_556 2_556
O11W Na2 O5W 102.2(13) . 2_557
O11W Na2 O8W 168.9(14) . .
O5W Na2 O8W 86.3(10) 2_557 .
O11W Na2 O3W 88.8(13) . 2_557
O5W Na2 O3W 90.4(11) 2_557 2_557
O8W Na2 O3W 83.9(10) . 2_557
O11W Na2 O6W 83.9(15) . .
O5W Na2 O6W 173.5(13) 2_557 .
O8W Na2 O6W 87.5(13) . .
O3W Na2 O6W 87.4(13) 2_557 .
O11W Na2 O35 90.3(12) . .
O5W Na2 O35 90.4(9) 2_557 .
O8W Na2 O35 96.9(10) . .
O3W Na2 O35 178.9(10) 2_557 .
O6W Na2 O35 91.8(13) . .
O11W Na2 Na6 126.2(13) . 2_667
O5W Na2 Na6 130.4(9) 2_557 2_667
O8W Na2 Na6 44.4(9) . 2_667
O3W Na2 Na6 81.5(9) 2_557 2_667
O6W Na2 Na6 43.2(11) . 2_667
O35 Na2 Na6 98.6(9) . 2_667
O31 Na3 O64 105.0(8) . 2_557
O31 Na3 Na6 99.2(8) . 1_445
O64 Na3 Na6 58.1(7) 2_557 1_445
O42 Na4 O1W 63.7(7) . .
O42 Na4 O56 144.2(11) . 1_655
O1W Na4 O56 127.3(10) . 1_655
O52 Na5 O67 106.0(10) . 2_567
O52 Na5 O1W 102.3(9) . 2_557
O67 Na5 O1W 144.3(12) 2_567 2_557
O52 Na5 O5W 97.6(10) . 2_557
O67 Na5 O5W 104.5(10) 2_567 2_557
O1W Na5 O5W 92.8(9) 2_557 2_557
O51 Na6 O9W 92.1(14) . .
O51 Na6 O6W 82.1(15) . 2_667
O9W Na6 O6W 90.9(17) . 2_667
O51 Na6 O8W 166.5(17) . 2_667
O9W Na6 O8W 81.6(15) . 2_667
O6W Na6 O8W 86.1(16) 2_667 2_667
O51 Na6 O51 85.7(12) . 2_667
O9W Na6 O51 171.2(16) . 2_667
O6W Na6 O51 97.2(16) 2_667 2_667
O8W Na6 O51 102.2(13) 2_667 2_667
O51 Na6 Na6 45.2(9) . 2_667
O9W Na6 Na6 136.6(18) . 2_667
O6W Na6 Na6 90.0(17) 2_667 2_667
O8W Na6 Na6 141.6(17) 2_667 2_667
O51 Na6 Na6 40.5(8) 2_667 2_667
O51 Na6 Na2 125.5(12) . 2_667
O9W Na6 Na2 82.3(12) . 2_667
O6W Na6 Na2 44.1(12) 2_667 2_667
O8W Na6 Na2 42.1(8) 2_667 2_667
O51 Na6 Na2 105.9(10) 2_667 2_667
Na6 Na6 Na2 124.9(13) 2_667 2_667
O51 Na6 W5 107.2(12) . 2_667
O9W Na6 W5 160.5(15) . 2_667
O6W Na6 W5 89.0(13) 2_667 2_667
O8W Na6 W5 78.9(10) 2_667 2_667
O51 Na6 W5 24.2(5) 2_667 2_667
Na6 Na6 W5 62.9(9) 2_667 2_667
Na2 Na6 W5 84.1(7) 2_667 2_667
O51 Na6 Na3 139.0(13) . 1_665
O9W Na6 Na3 107.7(13) . 1_665
O6W Na6 Na3 131.3(14) 2_667 1_665
O8W Na6 Na3 54.4(9) 2_667 1_665
O51 Na6 Na3 69.2(8) 2_667 1_665
Na6 Na6 Na3 103.8(12) 2_667 1_665
Na2 Na6 Na3 93.2(8) 2_667 1_665
W5 Na6 Na3 59.1(5) 2_667 1_665
O16W Na7 O4W 93.4(17) 2_556 .
O16W Na7 O13W 97.0(19) 2_556 2_556
O4W Na7 O13W 164.9(19) . 2_556
O16W Na7 O9 77.0(13) 2_556 2_556
O4W Na7 O9 83.3(12) . 2_556
O13W Na7 O9 88.5(15) 2_556 2_556
O16W Na7 Na1 87.4(13) 2_556 2_556
O4W Na7 Na1 40.5(8) . 2_556
O13W Na7 Na1 129.0(15) 2_556 2_556
O9 Na7 Na1 43.0(6) 2_556 2_556
Na7 O4W Na1 101.7(14) . 2_556
Na2 O5W Na5 129.8(11) 2_557 2_557
Na6 O6W Na2 92.7(17) 2_667 .
Na2 O8W Na6 93.5(13) . 2_667
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
W1 O71 1.76(2) .
W1 O43 1.85(2) .
W1 O59 1.854(17) .
W1 O69 1.969(17) .
W1 O29 1.993(17) .
W1 O46 2.422(16) .
W2 O66 1.65(2) .
W2 O29 1.849(19) .
W2 O65 1.881(16) .
W2 O19 1.932(17) .
W2 O60 1.937(17) .
W2 O46 2.315(15) .
W3 O67 1.759(18) .
W3 O35 1.754(16) .
W3 O68 1.92(2) .
W3 O60 1.941(17) .
W3 O59 2.045(18) .
W3 O46 2.244(14) .
W4 O57 1.694(19) .
W4 O48 1.820(15) .
W4 O54 1.835(18) .
W4 O45 1.930(16) .
W4 O43 1.96(2) .
W4 O22 2.366(16) .
W5 O51 1.717(15) .
W5 O64 1.723(18) .
W5 O68 1.94(2) .
W5 O53 2.021(17) .
W5 O48 2.089(18) .
W5 O22 2.227(14) .
W5 Na6 3.66(3) 2_667
W6 O61 1.71(2) .
W6 O69 1.882(17) .
W6 O33 1.899(15) .
W6 O45 1.910(17) .
W6 O10 1.997(18) .
W6 O47 2.300(15) .
W7 O52 1.695(19) .
W7 O49 1.737(17) .
W7 O19 1.904(17) .
W7 O7 1.908(14) .
W7 O30 2.265(15) .
W7 O58 2.301(15) .
W8 O62 1.735(15) .
W8 O30 1.809(16) .
W8 O10 1.931(19) .
W8 O50 1.939(15) .
W8 O65 1.975(16) .
W8 O47 2.201(15) .
W9 O63 1.742(16) .
W9 O28 1.785(17) .
W9 O53 1.870(16) .
W9 O13 1.967(14) .
W9 O54 2.090(17) .
W9 O22 2.279(15) .
W10 O1 1.755(14) .
W10 O36 1.790(14) .
W10 O15 1.875(15) .
W10 O20 1.951(14) .
W10 O44 2.144(14) .
W10 O18 2.246(13) .
W10 Dy2 3.5803(13) .
W11 O37 1.724(16) .
W11 O25 1.765(15) .
W11 O13 1.886(14) .
W11 O50 1.981(16) .
W11 O33 2.006(17) .
W11 O47 2.287(14) .
W12 O17 1.761(16) 2_557
W12 O32 1.755(12) .
W12 O41 1.801(15) .
W12 O31 2.040(14) .
W12 O3 2.089(13) .
W12 O27 2.241(14) .
W13 O40 1.727(15) .
W13 O26 1.831(13) .
W13 O5 1.870(14) .
W13 O6 1.906(15) .
W13 O16 2.095(13) .
W13 O23 2.323(14) .
W14 O39 1.715(14) .
W14 O44 1.749(15) .
W14 O24 1.844(15) .
W14 O4 1.948(15) .
W14 O26 2.105(13) .
W14 O23 2.303(14) .
W15 O56 1.740(16) .
W15 O3 1.818(14) .
W15 O12 1.953(14) .
W15 O38 1.955(13) .
W15 O5 2.004(14) .
W15 O27 2.346(14) .
W16 O34 1.756(16) .
W16 O31 1.863(14) .
W16 O20 1.869(14) .
W16 O24 1.941(14) .
W16 O12 1.946(14) .
W16 O27 2.327(13) .
W17 O55 1.782(15) .
W17 O42 1.783(13) .
W17 O72 1.783(13) .
W17 O15 2.054(14) .
W17 O8 2.140(12) .
W17 O18 2.289(14) .
W17 Dy2 3.5296(13) .
W18 O9 1.720(15) .
W18 O8 1.796(13) .
W18 O14 1.890(14) .
W18 O4 1.957(14) .
W18 O6 2.052(12) .
W18 O23 2.280(15) .
Sb1 O22 1.964(16) .
Sb1 O46 1.971(15) .
Sb1 O47 1.999(14) .
Sb2 O18 1.945(13) .
Sb2 O23 1.985(14) .
Sb2 O27 1.998(14) .
Sb3 O11 1.939(14) .
Sb3 O2 1.985(15) 2_557
Sb3 O58 2.015(14) .
Sb4 O11 2.007(14) .
Sb4 O16 2.175(14) .
Sb4 O14 2.176(14) .
Sb4 O7 2.240(14) .
Sb4 Dy1 3.4599(17) .
Sb5 O2 1.974(14) 2_557
Sb5 O16 2.019(13) .
Sb5 O38 2.114(14) .
Sb5 O7 2.207(15) .
Sb5 Dy2 3.5830(16) 2_557
Dy1 O72 2.263(13) .
Dy1 O21 2.309(15) .
Dy1 O28 2.329(16) .
Dy1 O17 2.312(15) .
Dy1 O14 2.374(14) .
Dy1 O25 2.434(15) .
Dy1 O11 2.492(14) .
Dy1 N1 2.522(12) .
Dy2 O41 2.291(15) 2_557
Dy2 O32 2.313(12) .
Dy2 O42 2.299(14) .
Dy2 O36 2.347(14) .
Dy2 O38 2.421(12) 2_557
Dy2 O2 2.496(14) .
Dy2 O1W 2.504(15) .
Dy2 O18 2.658(12) .
Dy2 Sb5 3.5831(16) 2_557
O2 Sb5 1.974(13) 2_557
O2 Sb3 1.985(15) 2_557
O9 Na7 2.46(3) 2_556
O9 Na1 2.511(19) .
O17 W12 1.761(16) 2_557
O21 C6 1.24(3) .
O21 Na1 2.457(16) .
O31 Na3 2.75(3) .
O35 Na2 2.57(2) .
O37 Na1 2.363(19) .
O37 Na1 2.87(2) 2_556
O38 Dy2 2.421(11) 2_557
O41 Dy2 2.292(15) 2_557
O42 Na4 2.76(3) .
O51 Na6 2.30(4) .
O51 Na6 2.51(4) 2_667
O52 Na5 2.70(3) .
O56 Na4 2.85(3) 1_455
O64 Na3 2.88(3) 2_557
O67 Na5 2.71(3) 2_567
O70 C6 1.26(3) .
O70 Na1 2.67(2) .
O1W Na4 2.77(3) .
O1W Na5 2.78(3) 2_557
N1 C1 1.390(9) .
N1 C5 1.390(9) .
C1 C2 1.390(9) .
C2 C3 1.390(9) .
C3 C4 1.390(9) .
C4 C5 1.390(9) .
C5 C6 1.46(2) .
C6 Na1 2.89(2) .
Na1 O4W 2.43(3) 2_556
Na1 O2W 2.45(2) 2_556
Na1 O37 2.87(2) 2_556
Na1 Na1 3.65(2) 2_556
Na1 Na7 3.67(3) 2_556
Na2 O11W 2.32(4) .
Na2 O5W 2.36(3) 2_557
Na2 O8W 2.42(3) .
Na2 O3W 2.49(3) 2_557
Na2 O6W 2.51(5) .
Na2 Na6 3.60(4) 2_667
Na3 O64 2.88(3) 2_557
Na3 Na6 3.90(4) 1_445
Na4 O56 2.85(3) 1_655
Na5 O67 2.71(3) 2_567
Na5 O1W 2.78(3) 2_557
Na5 O5W 2.89(3) 2_557
Na6 O9W 2.44(5) .
Na6 O6W 2.47(5) 2_667
Na6 O8W 2.52(4) 2_667
Na6 O51 2.51(4) 2_667
Na6 Na6 3.53(7) 2_667
Na6 Na2 3.60(4) 2_667
Na6 W5 3.66(3) 2_667
Na6 Na3 3.90(4) 1_665
Na7 O16W 2.25(5) 2_556
Na7 O4W 2.29(4) .
Na7 O13W 2.32(5) 2_556
Na7 O9 2.46(3) 2_556
Na7 Na1 3.67(3) 2_556
O2W Na1 2.45(2) 2_556
O3W Na2 2.49(3) 2_557
O4W Na1 2.43(3) 2_556
O5W Na2 2.36(3) 2_557
O5W Na5 2.89(3) 2_557
O6W Na6 2.47(5) 2_667
O8W Na6 2.52(4) 2_667
O13W Na7 2.32(5) 2_556
O16W Na7 2.25(5) 2_556
loop_
_platon_squeeze_void_nr
_platon_squeeze_void_average_x
_platon_squeeze_void_average_y
_platon_squeeze_void_average_z
_platon_squeeze_void_volume
_platon_squeeze_void_count_electrons
1 0.139 0.500 0.462 1226.4 789.9
2 0.485 0.947 0.553 18.7 11.7
3 0.514 0.053 0.447 18.6 13.9
